Re-entrant structural phase transition in a frustrated kagome magnet, Rb2SnCu3F12
Downie, Lewis J.; Thompson, Stephen P.; Tang, Chiu C.; Parsons, Simon; Lightfoot, Philip; CrystEngComm 15 (2013) 7426–; doi:10.1039/c3ce41422a

data_7215175
_publ_section_title
;
 Re-entrant structural phase transition in a frustrated kagome magnet,
 Rb2SnCu3F12
;
_journal_issue                   37
_journal_name_full               CrystEngComm
_journal_page_first              7426
_journal_paper_doi               10.1039/c3ce41422a
_journal_volume                  15
_journal_year                    2013
_chemical_formula_moiety         Rb2Sn1Cu3F12
_chemical_formula_sum            'Cu3 F12 Rb2 Sn'
_chemical_formula_weight         708.26
_chemical_melting_point          ?
_chemical_name_common            Rb2Sn1Cu3F12
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           148
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            12
_cell_length_a                   13.8749(10)
_cell_length_b                   13.8749(10)
_cell_length_c                   20.2458(14)
_cell_measurement_reflns_used    2537
_cell_measurement_temperature    245
_cell_measurement_theta_max      28.562
_cell_measurement_theta_min      3.53
_cell_volume                     3375.4(4)
_computing_cell_refinement
;
        CrysAlisPro, Agilent Technologies,
        Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
        (compiled Feb  1 2013,16:14:44)
;
_computing_data_collection
;
        CrysAlisPro, Agilent Technologies,
        Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
        (compiled Feb  1 2013,16:14:44)
;
_computing_data_reduction
;
        CrysAlisPro, Agilent Technologies,
        Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
        (compiled Feb  1 2013,16:14:44)
;
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      245
_diffrn_detector_area_resol_mean 5.1574
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.846
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Atlas'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0706
_diffrn_reflns_av_sigmaI/netI    0.0670
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            5911
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         28.86
_diffrn_reflns_theta_min         3.02
_exptl_absorpt_coefficient_mu    16.520
_exptl_absorpt_correction_T_max  0.397
_exptl_absorpt_correction_T_min  0.026
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
        CrysAlisPro, Agilent Technologies,
        Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
        (compiled Feb  1 2013,16:14:44)
Analytical numeric absorption correction using a multifaceted crystal
                        model based on expressions derived by R.C. Clark & J.S.
        (Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    4.181
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             3828.0
_exptl_crystal_size_max          0.5626
_exptl_crystal_size_mid          0.3079
_exptl_crystal_size_min          0.056
_refine_diff_density_max         1.092
_refine_diff_density_min         -1.503
_refine_diff_density_rms         0.292
_refine_ls_extinction_coef       0.00010(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.124
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     112
_refine_ls_number_reflns         1679
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.124
_refine_ls_R_factor_all          0.0707
_refine_ls_R_factor_gt           0.0515
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0395P)^2^+27.9746P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1101
_refine_ls_wR_factor_ref         0.1189
_reflns_number_gt                1367
_reflns_number_total             1679
_reflns_threshold_expression     >2\s(I)
_cod_data_source_file            c3ce41422a_3.cif
_cod_data_source_block
;
;
_cod_depositor_comments
;
The following automatic conversions were performed:

'_chemical_melting_point' value 'not measured' was changed to '?' -
the value is undefined or not given.

'_symmetry_cell_setting' value
'TRIGONAL' changed to 'trigonal' according to
/usr/data/users/saulius/automatic-downloads/retrospective/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        'Cu3 F12 Rb2 Sn1'
_cod_database_code               7215175